N° d’ordre : 2283
présentée pour obtenir
LE TITRE DE DOCTEUR DE L’INSTITUT NATIONAL POLYTECHNIQUE DE TOULOUSE &
THE TITLE OF DOCTOR OF PHILOSOPHY OF THE INSTITUTE OF CHEMICAL TECHNOLOGY, PRAGUE
École doctorale : Energétique et Dynamique des Fluides Spécialité : Energétique et transferts – Systèmes et Procédés
Par M. Jaroslav BLAŽEK
Titre de la thèse : - français
ETUDE DES SCHEMAS REACTIONNELS DE DEGRADATION THERMIQUE DES POLYMERES
- anglais STUDY OF THE REACTION KINETICS OF THE THERMAL
DEGRADATION OF POLYMER
- tchèque TERMICKÁ DEGRADACE ORGANICKÝCH MATERIÁLŮ
Soutenue le 11 Novembre 2005 devant le jury composé de :
M. Bohumil KOUTSKÝ Président
MM. Didier LECOMTE, Petr BURYAN Directeurs de thèse
André FONTANA, Pavel STRAKA, Ivan VÍDEN Rapporteurs
František HRDLIČKA Membre
Yannick SOUDAIS Membre
Florent LEMORT Membre
1. INTRODUCTION ... 11
2. THEORETICAL BACKGROUNDS ... 12
2.1 Pyrolysis ... 12
2.1.1 Various possible methods of use of plastic polymers... 14
2.2 Thermal analysis ... 17
2.2.1 Thermogravimetric analysis... 19
2.3 Kinetics ... 24
2.3.1 Isothermal vs. non-isothermal kinetics and other issues... 28
2.4 Polymers ... 37 2.4.0 Studied polymers... 48 2.4.1 Lignin ... 48 2.4.2 Cellulose... 60 2.4.3 EVA ... 62 2.4.4 PS ... 64 2.4.5 PVC ... 69
3. EXPERIMENTAL PART – STUDY OF THE KINETICS OF THE THERMAL DEGRADATION OF POLYMERS... 72
3.1 Materials and experimental apparatuses... 72
3.2 PART A – Kinetic study of the thermal degradation of polymers – isoconversional method (model-free method) ... 75
3.2.1 TGA data treatment ... 75
3.2.2 Kinetic model in literature ... 81
22.214.171.124 Lignin ... 81
126.96.36.199 Cellulose... 83
188.8.131.52 Ethylene vinyl acetate... 85
184.108.40.206 Polystyrene ... 89
220.127.116.11 Polyvinyl chloride ... 92
3.2.3 Analysis of experimental results ... 97
18.104.22.168 Lignin ... 97
22.214.171.124 Cellulose... 100
126.96.36.199 Ethylene vinyl acetate... 101
188.8.131.52 Polystyrene ... 103
184.108.40.206 Polyvinyl chloride ... 105
3.2.4 Discussion and conclusions ... 107
3.3 PART B – Kinetic study of thermal degradation of polymers – numerical resolution of kinetic equations obtained from reaction pseudo-schemes (model-fitting method) ... 111
3.3.1 Lignin ... 111
3.3.2 EVA ... 125
3.3.3 Study of the degradation kinetics of binary mixtures of polymers ... 135
3.3.4 Simulation of kinetic models in MatLab... 156
3.3.5 FTIR analysis of released gases... 166
3.3.6 Discussion and conclusions ... 178
4. DISCUSSION AND CONCLUSION ... 179
5. REFERENCES... 181
Appendix A: FTIR working protocol... 197
Appendix B: Experimental results, EVA kinetics... 200
Appendix C: Detailed description of the thermobalance ... 203
Appendix D: Description of the FTIR spectrometer... 206
Appendix E: Tables for Part 1 ... 208
Appendix F: Figures for Part 1... 219
Appendix G: Polymer generalities ... 257
Appendix H: List of publications and presentations of professional activities ... 259
Appendix I: Notation used... 261
List of figuresFig. 1: Plastic materials susceptible to recycling ... 14
Fig. 2: Industrial pyrolysing unit P.I.T. – PYROFLAM® with energy valorization ... 15
Fig. 3: Thermal conductivity of furnace atmosphere gases... 22
Fig. 4: Linear, branched, and network polymer configuration... 39
Fig. 5: Chain polymerization and step polymerization... 43
Fig. 6: Free-radical polymerization: example of styrene... 44
Fig. 7: Polystyrene prepared by free-radical polymerization... 44
Fig. 8: Polymerization of terephthalic acid and ethylene glycol... 45
Fig. 9: Polyethylene terephthalate ... 46
Fig. 10: Cut through a young black conifer... 49
Fig. 11: Lignin monomer (coniferine and syringine) ... 50
Fig. 12: Formulae of three principal lignin alcohols ... 50
Fig. 13: Lignin polymerisation. R1, R2 = H or OCH3... 51
Fig. 14: Types of bonds that occur in lignine ...51 and 52 Fig. 15: Model of lignin based on coniferyne ... 53
Fig. 16: Model of lignin based on syringine... 54
Fig. 17: Kraft extraction process... 56
Fig. 18: Sulfite extraction ... 57
Fig. 19: Sulfonation of Kraft lignins ... 59
Fig. 20: Chemical formula of cellulose... 60
Fig. 21: Principal cellulose monomer ... 60
Fig. 22: Chemical formula of EVA ... 62
Fig. 23: Elementary motive of polystyrene molecule – styrene... 67
Fig. 24: Radical polymerisation of styrene into PS ... 68
Fig. 25: Reaction of synthesis of polyvinyl chloride ... 70
Fig. 26: Distribution of various materials used in conditioning of drinking waters ... 70
Fig. 27: Experimental apparatuses ... 73
Fig. 28: Temperature sensor location ... 74
Fig. 29: Cellulose depolymerisation scheme ... 83
Fig. 30: Scheme of the 1st stage of the EVA decomposition ... 87
Fig. 31: Scheme of the reactions of the second stage of the EVA decomposition – formation of transvinyls and disproportionation of free radicals... 87
Fig. 32: Formation of lacton (a), formation of ketones and acetaldehyde (b) ... 88
Fig. 33: Influence of temperature on PS degradation products ... 90
Fig. 35: Reaction order as a function of temperature ... 121
Fig. 36: Frequency factor as a function of temperature... 121
Fig. 37: Activation energy as a function of temperature ... 122
Fig. 38: A simple graphical representation of appearance of TGA/DTA charts obtained by pyrolysis of EVA... 125
Fig. 39: Mass loss rates as a function of time for different types of EVA. These results are extrapolated from the model for all types of EVA... 127
Fig. 40: Relative mass loss curves (EVA + EVA*) represented in function of time and defined (parameterised) by VA percentage... 132
Fig. 41: On the same model as the preceding curves, this one represents the mass loss for the single EVA (the first stage)... 123
Fig. 42: Points corresponding to the table of calculations of VA percentage in order to visualise errors in function of EVA type considered for modelling ... 133
Fig. 43: Relative errors as a function of VA percentage... 134
Fig. 44: CEA personnel in the middle of manipulating plutonium with plastic gloves ... 135
Fig. 45: Representation of mass in time for EVA/PS mixture (25/75 ratio) for the heating rate of 10 °C.min-1 . N.B.: Experimental mass is in green, theoretical in blue... 145
Fig. 46: Representation of mass variations in time for EVA/PS mixture (25/75 ratio) at the heating rate of 10 °C.min-1 ... 146
Fig. 47: Superposition of TGA curves for pure EVA, pure PVC, and the mixture of both, at three different ratios (X-Y %, where X stands for EVA, and Y stands for PVC) ... 153
Fig. 48: Kinetic scheme of EVA degradation... 156
Fig. 49: Mathematical expression of the kinetic model of EVA pyrolysis ... 156
Fig. 50: Comparison of experimental and calculated curves for pure PVC ... 157
Fig. 51: Kinetic scheme of PVC degradation... 157
Fig. 52: Kinetic model of PVC expressed mathematically... 158
Fig. 53: Broido-Schafizadeh reaction scheme ... 158
Fig. 54: Comparison of the experimental and calculated curve for the pure cellulose pyrolysis... 160
Fig. 55: Comparison of experimental and calculated curve for EVA/PVC mixture ... 161
Fig. 56: Comparison of experimental and calculated curves for EVA/Cellulose mixture pyrolysis... 163
Fig. 57: Superposition of TGA experimental curves of pure cellulose, pure EVA and of the mixture of both ... 164
Fig. 58: Gram-Schmidt of pure EVA ... 169
Fig. 59: Absorption spectrum during the EVA degradation at 1,006.87 s ... 170
Fig. 60: Characteristic spectrum of acetic acid ... 170
Fig. 61: Absorption spectrum during the degradation of EVA at 1,579.19 s... 171
Fig. 62: Gram-Schmidt of the pure PVC ... 172
Fig. 63: Characteristic transmitance spectrum (= 1 - absorbance) of HCl ... 172
Fig. 64: Absorption spectrum during the PVC degradation at 922.6 s ... 173
Fig. 65 : Gram-Schmidt of EVA/PVC mixture ... 174
Fig. 66: Absorption spectrum during the degradation of the EVA/PVC mixture at 785.23 s ... 174
Fig. 67: Absorption spectrum for the degradation of EVA/PVC mixture at 785.23 s... 175
Appendix C Fig. C-1: Thermogravimetric unit TGA 92... 203
Fig. C-2: Microbalance B92 ... 204
Fig. D-1: Michelson interferometer... 207
Appendix F Figs. F-1 to F-3: Lignin TGA curves, α = f(t) relation, t = f(τ) chart ... 219
Fig. F-4: Lignin TGA and DTG detailed chart... 222
Figs. F-5 to F-7: Cellulose TGA curves, α = f(t) relation, t = f(τ) chart... 223
Fig. F-8: Cellulose pyrolysis calculated Eas’ diagram ... 226
Figs. F-9 to F-11: EVA “12” TGA curves, α = f(t) relation, t = f(τ) chart... 227
Fig. F-12: EVA “12” pyrolysis α = f(t) selected values chart ... 230
Figs. F-13 to F-19: EVA “12” best kinetic model charts, F = f(1/β)... 231
Figs. F-20 to F-23: EVA “25” TGA curves, α = f(t) relation, t = f(t), and α = f(t) selected values charts ... 238
Figs. F-24 to F-30: EVA “25” best kinetic model charts, F = f(1/β) ... 242
Fig. F-31: EVA “12” and “25” – VA percentage influence on degradation compared ... 249
Figs. F-32 to F-35: PS TGA chart, TGA curves in detail, α = f(t) relation, and t = f(τ) charts... 250
Figs. F-36 to F-38: PVC TGA curves, α = f(t) relation, t = f(τ) chart ... 254
Appendix G Fig. G-1: Consumption of thermoplastics in Europe in 2000 and 2001 ... 257
Fig. G-2: Consumption of thermoplastics in Europe in 2001 ... 257
List of tablesTab. 1: Principal thermoanalytical methods... 19
Tab. 2: Types of polymerization reactions [TRP Project] ... 46
Tab. 3: World annual production of different types of lignin ... 57
Tab. 4: Properties of lignosulfates and kraft lignins ... 59
Tab. 5: Identity card for styrene... 67
Tab. 6: Identity card for vinyl chloride... 71
Tab. 7: Used sample materials ... 72
Tab. 8: Analytical forms of various conversion functions ... 80
Tab. 9: Kinetic parameters of lignin pyrolysis (various sources)... 82
Tab. 10: Kinetic parameters of PS decomposition ... 91
Tab. 11: Kinetic parameters of PVC pyrolysis [Marcilla & Beltrán 1995a] ... 93
Tab. 12: Kinetic parameters of PVC pyrolysis [Miranda et al. 1999]... 96
Tab. 13: Lignin IR absorption bands [Hergert 1971] ... 98
Tab. 14: Results obtained by Pascali and Herrera, n and A as a function of t ... 112
Tab. 15: TGA kinetic analaysis values by Pasquali and Herrera ... 112
Tab. 16: Comparison of literature and experimental results... 115
Tab. 17: Results of the simulation ... 117
Tab. 18: Kinetic parameters for isothermal experiments with lignin... 120
Tab. 19: Kinetic parameters for EVA... 126
Tab. 20: Initialization parameters of the optimization programme ... 129
Tab. 21: Values of frequency factor and activation energy ... 129
Tab. 22: Calculation of VA percentage form plateau pitches ... 133
Tab. 24: Results (temperature and DTG) of PS (single) pyrolysis... 138
Tab. 25: Recap of graphical observations of experimental curves for EVA/PS mixture... 139
Tab. 26: Selection of parameter initialisation values ... 143
Tab. 27: Example of table with results obtained in MatLab for EVA/PS mixture in 25/75 ratio, respectively, and at 10 °C.min-1 ... 144
Tab. 28: Relative errors of frequency factors and activation energy values ... 144
Tab. 29: Table of relative errors of mass data ... 146
Tab. 30: Chronological disappearance orders of reactants and reaction intermediates ... 147
Tab. 31: Mass loss, DTG, and DTG peak temperature values for pure EVA... 150
Tab. 32: Mass loss, DTG, and DTG peak temperature values for pure PVC... 150
Tab. 33: Mass loss, DTG, and DTG peak temperature values for pure pyrolysis... 151
Tab. 34: Mass loss, DTG, and DTG peak temperature values for EVA/PVC mixture... 151
Tab. 35: Mass loss, DTG, and DTG peak temperature values for EVA/Cellulose mixture152 Tab. 36: Maximal relative errors of the mass loss from the correlation of experimental and calculated curves... 162
Appendix B Tab. B-1: Results for EVA from simulations ... 200
Appendix E Tab. E-1 to E-2: Lignin pyrolysis frequency factors and activation energies calculated .. 208
Tab. E-3 to E-4: Cellulose pyrolysis frequency factors and activation energies ... 209
Tab. E-5 to E-10: EVA pyrolysis frequency factors and activation energies ... 210
Tab. E-11 to E-17: PS pyrolysis frequency factors and activation energies ... 213
Tab. E-18 to E-21: PVC pyrolysis frequency factors and activation energies ... 216
Appendix G Tab. G-1: Consumption of thermoplastics in Europe... 257
Firstly I must express my appreciation to my Czech thesis director Prof. Ing. Petr Buryan, DrSc. and Ing. Viktor Tekáč who fostered me throughout the whole thesis, as well as all other members of the Department of Gas, Coke and Air Protection of the Institute of Chemical Technology in Prague.
Prof. Didier Lecomte, my French thesis director, has always been ready to lend me a helping hand. Prof. Didier Grouset has given me some good tips to make my thesis more sound and complete. And every credit for the organizational success of the thesis goes to Dr. Yannick Soudais, who was at the same time the initiating factor of the thesis. Expert laboratory assistant Ludivine Moga has often spontaneously come with new ideas how to enhance quality of data treatment by modifying the output of machines. My thanks are to the entire team of the Centre énergetique-environnnement of the Ecole des Mines d’Albi-Carmaux, for their encouragement and suggestions.
Next are my thanks aimed unto Miguel Sanchez Amoros (Universidad Politécnica de Cartagena) and Daniel Barrabes Pradal (Escola Tècnica Superior d’Enginyers Industrials de Barcelona) for their assistance in FTIR analyses; and Shan Jiang (Ecole des Mines d’Albi-Carmaux) for his calculations in Sidolo.
Special acknowledgements are expressed to the French Embassy in Prague, which has offered the possibility to launch this joint thesis project and provided the consecutive support in the practical implementation of the thesis by enabling to benefit from the grant by the French government, in the programme BGF (bourse du gouvernement français).
A part of the study was cofinanced by CEA (Commissariat à l’Energie Atomique, i.e. the French Atomic Energy Commission), SCDV (Service de Conditionnement des Déchets et Vitrification). Appreciation of this fact is expressed as well.
Disertační práce se zabývá pyrolýzou polymerů za atmosférického tlaku, v oblasti teplot 20-1000°C.
Teoretická část práce uvádí historické mezníky ve vývoji termické degradace polymerů a přehledně shrnuje současný stav problematiky. Nadto obsahuje základní poznatky týkající se metod výroby polymerů a v několika tabulkách seznamuje s průmyslovou produkcí těchto materiálů v Evropě.
Cílem experimentální práce bylo ověřit možnost aplikace specifické metody k výpočtu kinetických parametrů pyrolýzy (aktivační energie a frekvenčního faktoru) a jejich porovnání s údaji uváděnými v literatuře.
Experimenty byly prováděny v laboratorním měřítku. Byl použit termogravimetr sériově napojený na spektrometr FTIR. Výstupními údaji byl úbytek hmotnosti v korelaci s narůstající teplotou. Množina spekter odpovídajících různým stádiím pyrolýzních experimentů podpořila předpokládané mechanizmy rozkladu.
K výpočtu kinetických parametrů pyrolýzy polymerů byla použita integrální metoda Ozawa-Flynn-Wall a metoda využívající speciálního programu vytvořeného za tímto účelem v programu MatLab. Potřebné kinetické parametry byly získány pomocí „solverů“ (rutin) využívajících soustavy diferenciálních rovnic. Výsledky obou metod byly porovnány.
Sledovanými polymery byly dva „přírodní polymery“ – lignin a celulóza, a průmyslově připravené polymery: EVA, PS a PVC. Ve většině případů byla konstatována velmi dobrá shoda s kinetickými parametry nalezenými v dostupné literatuře.
Vypočtené hodnoty aktivační energie jsou v rozsahu od 118 kJ.mol-1, std. odch. 2,73 kJ.mol-1, (první fáze degradace PVC) do 454 kJ.mol-1, std. odch. 78,1 kJ.mol-1 (pyrolýza ligninu). Hodnoty frekvenčního faktoru se nacházejí v rozmezí od 7,66.109 s-1, std. odch. 1,58.109 s-1 (Difuzní model 3), a to pro 1. stupeň degradace PVC, do 1,84.1045 s-1 pro Model F1 (řád reakce = 1), std. odch. 5,5.1045 s-1 pro pyrolýzu ligninu. Vypočtené hodnoty pyrolýzy ligninu vykazovaly jisté zvláštnosti. Další hodnotou frekvenčního faktoru je 1,77.1022 s-1, std. odch. 8,22.1021 s-1 pro druhé stádium degradace „EVA 25“ (řád reakce = 1).
Detailní studium pyrolýzy binárních sloučenin EVA/PVC, EVA/PS a EVA/celulóza, doprovázena analýzou uvolněných plynných termodegradentů pomocí spektrometrie FTIR přispěla lepšímu pochopení pyrolýzních jevů a byla uplatněno i k řešení problémů v průmyslovém měřítku.
Předkládaná disertační práce je součástí spolupráce Vysoké školy chemicko-technologické v Praze a Institut National Polytechnique de Toulouse, v rámci programu Doctorat en cotutelle (společně řízená doktorská práce), financovaného z prostředků francouzské vlády. Experimentální práce byly uskutečněny převážně na Ecole Nationale Supérieure des Techniques Industrielles et des Mines d’Albi-Carmaux.
Accumulation of various plastic wastes begins to pose a serious problem. By creating waste sites, valuable chemical raw materials are lost. Moreover, in many countries, laws and regulations are fighting disposal of used plastic materials. Therefore, other solutions such as thermal treatment have to be taken into account.
Destruction of wastes by means of thermal treatment (combustion, pyrolysis) very often leads to pollution of the atmosphere by toxic pollutants as e.g. HCl, HCN, NOX, SO2, fly ash, compounds of the type of PCDD and PCDF. However, the pyrolysis process allows recovery of chemical products and energy from wastes.
The actual level of knowledge or state of arts, as well as the sustainability approach, do not allow us to adopt any new technology without considering its influence on our environment. It is therefore necessary to eliminate the production of toxic compounds. For this to be done effectively, understanding of the reaction pathways of polymer pyrolysis is vital. Thus, the best concepts and methods of the elimination of pollutants can be found and chemical resources as well as energy can be obtained. Using this information, processes may be designed for better control of flue gases and chemical compounds as well as energy consumption or recovery.
2. Theoretical backgrounds
Pyrolysis and thermolysis, commonly referred to as destructive distillation, are defined as an irreversible chemical change brought about by the action of heat in an oxygen-deficient (less than 2 %), inert-gas environment. The pyrolysis process requires temperatures ranging from 400 °C to 900 °C. Pyrolysis systems use a source of heat to drive the endothermic pyrolysis reactions in the complete absence of oxygen. The only difference between pyrolysis and thermolysis is that the former employs a direct heat source within the reactor (retort), while the latter employs an indirect external source of heat to the reactor (retort). Depending on particular reaction conditions (temperature, partial pressure of oxygen, total pressure), the organic fraction decomposes into gas, oil, and solid carbonaceous residues. Mild temperatures favour production of oils against gases. These products are recuperated at the end of the process, with the intention of being valorised.
Low oxygen content can be obtained under partial vacuum, by reinjecting one part of produced gases in the reactor or by injecting gaseous nitrogen into input riddle. The thermolysis technologies differ from each other by the reactor type, methods of reactor heating and conversion operating conditions.
Pyrolysis leads to decomposition of matter into various by-products (gas, oil, char, etc.). Yields of particular products are very variable, according to pyrolysis technology used. Some processes lead only to gases, others will produce a great quantity of oil. Pyrolysis products are gas, liquid, and char, the relative proportion of which depend very much on the pyrolysis method and process. Pyrolysis products are synthetic gas, oil, and carbonaceous residue. Synthetic gas produced in pyrolysis consists generally of a mixture of volatile organic compounds, some more heavy than others, methane, hydrogen, carbon dioxide and monoxide, and water coming largely from a humid fraction of the waste. After its treatment, gas can contain yet more volatile organic compounds (oil or tar). Most often, it is valorised in a boiler or directly in a thermolysis reactor, producing energy necessary for the thermal dissociation.
Oil is produced by condensation of a fraction of synthetic gas. Liquid thus obtained is refined by extraction and catalysis and then energetically valorised. Oil is an interesting product because it enables storage of energy that can be consequently used in a combustion turbine or a diesel engine.
Carbonaceous residue is a material relatively akin to lean coal, containing between 10 and 40 % of carbon. It can be valorized in situ in a classical boiler to give heat. The final residue is thus composed of fly ash from coal combustion. Some systems use a gasification stage to convert coal into synthetic gas. Carbonaceous residue can also be forwarded to a thermal power station or a cement factory and valorized ex situ.
Plastic materials cover a considerable spectrum of applications in our daily life. In France, in connection with evolution of legal regulations concerning waste sites, there cannot be used dumping for wastes, beginning the 1st of January 2002. They must be treated otherwise, e.g. by pyrolysis.
Pyrolysis is an alternative process of reuse of plastic materials to incineration and recycling. Recycling is being encouraged – it is compulsory for the EU members to recycle a minimum of 25 % and a maximum of 45 % of the total waste. By chemical recycling, plastic wastes can be converted to chemical feedstock, which can be used to produce new valuable products. Nevertheless, chemical recycling has the drawback of high-energy demand, and furthermore non-catalytic thermal degradation of polyolefin results in a wide range of products. Thus, pyrolysis seems to be an environmentally friendly process; yet, there are some disadvantages associated with it. The energy consumption is high and the molecular weight distribution of the products obtained tends to be quite broad, depending on the conditions used. The products can be used mostly as a low quality combustible. Elevated operating costs and the costs involved in the separation of the complex mixture lower the economical attractiveness of the process.
Pyrolysis (thermal cracking) of plastic waste allows recovering monomers and other petrochemical products. It is possible to obtain a mixture of hydrocarbons working at atmospheric pressure and moderate temperatures (500-850°C). During this process, quite a small gas volume can be obtained compared to incineration [Escola 1998]. Moreover, metallic toxic products are concentrated in the ashes, thus preventing undesirable emissions.
Howbeit, in the last few years the catalysed pyrolysis of plastics is being considered as a chance to avoid the problems mentioned above. However, this is not feasible without a perfect mastering of the kinetics of degradation for each and every polymer and all their possible mixtures, i.e. understanding their kinetic schemes and in parallel evaluating their thermodynamic parameters as well. It is imperative to know energy balances, released gases, products, by-products, … In this perspective, development of pyrolysis should be favoured.
Therefore, it has become interesting to know pyrolysis behaviour of certain number of polymers. And finally, in the domain of medical wastes, or even nuclear wastes, pyrolysis has to be preferred.
The study of kinetics and the knowledge of the main evolved gases are the main objectives of the present thesis.
2.1.1 Various possible methods of use of plastic polymers
According to the obligation in matter of wastes with the 2002 deadline, plastics cannot be from now on put on dumping sites. First of all, they must be treated by some method. However, the method of recycling depends on their nature and source.
There are 4 main techniques of recycling and valorisation of wastes:
Thermal recycling by combustion (incineration) methods. This one is applied on mixed and unsorted wastes. The generated energy is thus in the form of calorific energy. In fact, combustion of polymers, particularly plastic materials (in which 60 % constitute carbon and hydrogene) produces a lot of heat. For example, plastic materials, representing approx. 10 % of domestic waste, deliver 50 % of heat of incineration.
Physical recycling by collection of pure thermoplastic wastes. They are reprocessed and enter again into the process of transformation of plastic materials. Certain mixtures of plastic wastes are combined with other materials to give composite materials as e.g. those which serve to be formed into public benches.
Chemical recycling consists in chemical treatment of wastes with aim of obtaining basic molecules of chemical industry. This method, analogously to pyrolysis, grows up to be developed more and more in future. It could even become an unfailing and regular supply of raw materials.
Pyrolysis (breaking of certain bonds under the effect of heat) is heating of a material in an inert atmosphere. In comparison with combustion (thermal degradation in the presence of air), lower temperatures (from 400 to 700°C) is generally used.
Generated products are: oily residue that is composed of organic products (it is also called synthetic oil); tar; combustible gases with enhanced calorific properties.
In the case of polymers, these products can be valorised in the form of reusable energy, but also in the form of recyclable products.
The figure on the next page (Fig. 2) presents the P.I.T. Pyroflam pyrolysis process unit by Serpac Environnement. It is a gasification process aimed at the valorisation and conversion to energy of various solid wastes, including municipal solid wastes, industrial wastes, sludges, animal and meat wastes. The reactor comprises two chambers that rotate around a common horizontal axis on a slight incline. The waste pyrolysis chamber is cylindrical and the char gasification reactor is in the form of a truncated cone.
2.2 Thermal analysis
A typical method of investigating degradation kinetics of a pyrolysed substance is to measure its mass evolution in time, and commensurate with temperature.
In the present work, the problem of the influence of heat on polymers will be treated. The word analysis comes from the greek
η αναλυσις, solution of a problem. The word thermal comes from the greek
το θερµον, heat. Hence, the expression “thermal analysis” (TA) means literally the resolution of the heat problem.
The first documented thermogravimetric (TG) experiments were carried out in 1887 by Le Chatelier [Ozawa 2000]. The next pioneering work was done by Nernst & Riesenfeld , who used a Nernst quartz torsion microbalance, equipped with an electric furnace, to study the mass-loss on heating of Iceland spar, opal, zirconia, and other minerals. The method of differential thermal analysis (DTA) was invented in 1899. The so-called “French school of thermogravimetry” began with Urbain , when he modified a two-pan analytical balance into a crude thermobalance. In 1915, Japanese physicist Honda invented another thermogravimetric technique. Back then, the TA was used for materials such as minerals, metals, ceramics, inorganic compounds and refractory materials. Generally, two persons had to tend the machine and register data.
A fully automated TA apparatus was commercially available at the end of the years 50 of the previous century. The “First International Conference on Thermal Analysis” was held in 1965 in Aberdeen, Scotland.
The currently accepted definition of thermal analysis, as given by Mackenzie  and the International Confederation for Thermal Analysis and Calorimetry (ICTAC) is: “A group of techniques in which a physical property of a substance and/or its reaction products is measured as a function of temperature whilst the substance is subjected to a controlled temperature program.”
As the definition implies, there are three criteria to be satisfied in order that a thermal technique be regarded as thermoanalytical:
1. A physical property has to be measured;
2. This measurement has to be expressed as a function of temperature; 3. And it has to be done under a controlled temperature program.
The measured physical property and the corresponding thermal analysis technique are cited in Table 1. Note that the technique called “Emanation thermal analysis” (ETA) and “Thermoparticulate analysis” could well be inserted into the category of techniques used to measure mass. As can be seen in the table, other properties that can be determined by means of thermal analysis, in addition to direct thermal properties, are e.g.: mechanical properties (thermal expansion, softening, …), catalysis, corrosion, phase transformations and equilibriums.
As Wendlandt , Liptay  or Dunn  observe in their surveys of the types of thermal analysis techniques used and their applications in numerous areas of research, the most widely used techniques are TG and DTA, followed by DSC and TMA. Materials that are the most frequently studied are inorganic ones, high polymers, metals and metallic alloys, and organic substances. Thermal analysis is used for supportive research relating to quality control, troubleshooting and for innovative research into processes, base materials, materials and products. According to Lombardi , there were some 10,000 thermoanalytical instruments used throughout the world at the outset of 1990s.
Thermal analysis has become the most frequently used polymer characterization method.
Prior to 1969-1970, thermal analysis papers were published in a large number of international scientific journals, making a literature search very time-consuming, as notes Wendlandt . In 1969, the Journal of Thermal Analysis was founded by Buzagh and Simon in Hungary. In 1970, the Thermochimica Acta journal was founded (by Wendlandt). As an illustration of the growth of publications on the subject matter of thermal analysis, it can be mentioned that the Thermochimica Acta has increased its volume from about 400 pages in 1970 to over 3600 pages in 1983. Two useful abstracting journals are available: Thermal Analysis Abstracts (Heyden & Sons, London), and Chemical Abstracts CA Selects: Thermal Analysis (Chemical Abstracts Service, Columbus, Ohio, USA).
In the present outline, the state of the arts of thermal analysis will be briefly discussed with a focus on recent literature. For a more detailed description of the historical developments and reflections about possible future trends, the article of Mathot  is recommended.
Tab. 1: Principal thermoanalytical methods (after Turi , Brown , Mathot ).
Measured property Name of the technique Abbreviation
Mass Thermogravimetry TG
Derivative thermogravimetry DTG
Evolved gas detection EGD
Evolved gas analysis EGA
Temperature Differential thermal analysis DTA
Enthalpy Differential scanning calorimetry DSC
Mechanical properties Thermomechanical analysis TMA
Dynamic mechanical analysis DMA
Optical properties Thermoptometry
Magnetic properties Thermomagnetometry TM
Electrical properties Thermoelectrometry
Acoustic properties Thermosonimetry TS
Evolution of radioactive gas Emanation thermal analysis ETA
Evolution of particles Thermoparticulate analysis TPA
2.2.1 Thermogravimetric analysis (TGA)
The change in sample mass in the TG is determined as a function of temperature and/or time. Three modes of thermogravimetry are found to be used in literature: (a) isothermal thermogravimetry, in which the sample mass is recorded as a function of time at constant temperature, (b) quasi-isothermal thermogravimetry, in which the sample is heated to some constant temperature, (c) dynamic thermogravimetry, in which the sample is exposed to the effect of some temperature programme, usually a linear rate.
The mass-change versus temperature curve that results from such experiments has various synonyms, e.g.: thermolysis curve, pyrolysis curve, thermogram, thermogravimetric curve, thermogravigram, thermogravimetric analysis curve, and so on. It gives us information concerning the characteristic of the sample in question, as are the thermal stability and composition of the initial sample or any intermediate compounds that can be formed, and the composition of the possible residue as well.
The characteristic magnitudes of any single-stage nonisothermal reaction are two temperatures: the initial temperature Ti (sometimes called also the procedural decomposition temperature, pdt), defined as the temperature at which the cumulative change of mass reaches a value that the thermobalance can detect; and the final
temperature, Tf, which is the temperature at which the cumulative change of mass first reaches its maximum value, corresponding to complete reaction. At a linear heating rate, Tf is necessarily greater than Ti; the difference Tf – Ti, is called the reaction interval. For an endothermic decomposition reaction, Ti and Tf both increase with increasing heating rate, the effect being greater for Tf rather than for Ti.
Some factors affecting thermogravimetric experiments
There is a large number of factors, which affect the nature, precision, and accuracy of the experimental results in TG. Basically, the factors fall into the following two categories: 1. Instrumental (thermobalance) factors, 2. Sample characteristics.
Of course, many of these factors are fixed with a given thermobalance. And also because of the diversity in sample materials, it is difficult to reproduce such variable factors as the sample-particle size, the sample packing, furnace convection currents, and electrostatic effects, to mention the most significant. Unfortunately, some type of standard sample is not available to compare one given experimental apparatus with another.
Now some instrumental factors will be glanced upon. To begin with, the effect of the rate of heating will be considered. For a single-stage endothermic reaction, Simons and Newkirk  have pointed out the following changes for Ti and Tf, as a function of fast (F), and slow (S) heating rates. For the initial procedural decomposition temperature, (Ti)F > (Ti)S. For the final procedural temperature, (Tf)F > (Tf)S, while the reaction interval is characterized by the following term: (Tf–Ti)F > (Tf–Ti)S.
For any given temperature interval, the decomposition is greater at a low rate of heating than for a similar sample heated at a faster rate [Wendlandt 1986]. If the reaction involved is exothermic, the sample temperature will rise above that of the furnace, and Coats & Redfern  have shown that the difference between the furnace temperature and the sample temperature is greatest for the faster rate of heating when a reaction is occurring.
When successive reactions are involved, the rate of heating may well determine whether or not these reactions will be separated on the TG curve. The appearance of
a point of inflection at a faster heating rate may resolve itself into a horizontal plateau at a slow heating rate.
If a small sample is used, very fast heating rates may be employed and one will still be able to detect the presence of intermediate compounds formed during the decomposition reaction.
Now, the term “very fast heating rate” may correspond to various absolute values of heating rate, depending on the sample material used and other experimental conditions. However, one experiment that was taken as an instance justifying the conclusion remembered in the previous paragraph can be mentioned. In Perkin-Elmer Thermobalance brochure, a fast heating rate of 160° C.min-1 was used for the experiment with CuSO4×5H2O (2.37 mg, in a N2 atmosphere).
Nevertheless, as Popescu  confirms, the higher the heating rate, the more the heat transmission effect through the walls of the crucible plays a role; one looses the reaction information due to this. In particular, for pyrolysis experiments of the type used in our study, he recommends, as a general rule, heating rates inferior to 20 K.min-1. He advises to combine heating rates from 20 K.min-1 with sample weights of less than 10 mg.
Results of DeClerq & Duval  indicate that when samples containing a large amount of water are studied, a slow heating rate should be employed. Otherwise, inflection points can be made undistinguishable, as mentioned earlier. However, as Lukaszewski & Redfern  have observed, a sudden inflection in the mass-loss curve may be caused by a sudden variation in the rate of heating and thus be false. To detect this phenomenon, furnace temperature as a function of time should always be recorded.
As far as the effect of furnace atmosphere is concerned, it depends on the type of reaction, the nature of the decomposition products and the type of atmosphere employed. Different types of reactions can be met with, taking into account both the condition of original substances and products and the reversibility or irreversibility of reactions. In the field of thermogravimetric analysis, a dynamic (flowing) gas atmosphere is recommended, as the static (fixed) atmosphere implies changes of the gas concentration around sample that are virtually unquantifiable, thus making any attempts to attain reproducible results fruitless.
Moreover, the inert and oxidative types of atmosphere are being distinguished. Oxidation reactions can have effect on the mass-loss curve in both senses.
The rate of reaction is also dependent on how quickly heat is supplied to the system. Figure 3 below shows the thermal conductivity of He, N2, and Ar as a function of temperature (according to Caldwell et al. ).
Apparent mass gains are occasionally observed in the thermal decomposition of a sample under high vacuum conditions, if the sample layer is of a critical thickness and if a certain type of sample holder is employed.
Brown et al.  report opposite effects to those encountered in low-pressure atmosphere when high-pressure is used.
Numerous other studies on the effect of furnace atmosphere are available by Newkirk , Paulik and Paulik , etc.
0 10 20 30 40 50 60 70 80 90 0 200 400 600 800 1000 1200 t [°C] T h e rm a l co n d u ct iv it y [c a l. s -1 .c m -1 .°C -1 × 1 0 3 ] He N2 Ar
Fig. 3: Thermal conductivity of furnace atmosphere gases.
Sample holders range from flat plates to (deep) crucibles of various capacities. Materials used in their construction vary from glass, alumina, and ceramic compositions to various metals and metallic alloys. Newkirk & Aliferis  have shown that sodium carbonate
can react with porcelain or alumina crucibles at high-temperatures, thus producing a mass loss. The catalytic properties of platinum were reported by Ramakrishna et al.  to affect TG curves of certain metal sulfides.
Regarding the sample characteristics, the most important property is the amount of sample.
The sample masses can affect thermogravimetric experiments mainly in three ways, as Coats and Redfern  report it:
a) the endothermicity or exothermicity of reactions will cause the sample temperature to deviate from the temperature programme of TGA apparatus; this effect aggravates with increasing sample masses;
b) the diffusion conditions of the product gas around the solid sample particles; a convenient gas flow, rather than static conditions, does not allow the atmosphere immediately surrounding the reacting particles to be governed by the bulk of the sample;
c) the thermal gradients in the sample, increasing with its low thermal conductivity. Another aspect that could be taken into consideration is the size of sample particles. Generally, a decrease in particle size of the sample lowers the temperature at which thermal decomposition begins, and also the one at which it is completed. A sample consisting of large crystals or particles will often decompose more slowly than a sample of equal mass but consisting of very small particles; undoubtedly, the ratio of surface areas/mass is playing its role in this phenomenon.
Other properties are the nature of sample, heat of reaction, thermal conductivity, solubility of evolved gases in sample, etc.
Discussion on the above mentioned factors would not be more expanded. In the next chapter, the main subject matter will be presented.
The term kinetics derives from the ancient greek (
η κινησις, action of moving or moving oneself, movement, change). Used in the modern chemistry language, it designates the study of the reaction rate of chemical or enzymatic reactions.
Chemistry and kinetics of the thermal degradation of hydrocarbons is important in several different domains of process and environmental engineering. These are e.g. geochemistry, conversion of petroleum, coal, and biomass to liquid fuels, cracking processes, and recycling of polymers.
The kinetics of polymer decomposition can be studied in order to determine the appropriate conditions for hindering or limiting the evolution of toxic compounds and recuperation of raw materials from the thermal treatment of plastic wastes.
The principal objectives common to the majority of kinetic studies are the determination of the rate equation, i.e. the description of the extent of conversion of reactant(s) or formation of product(s) with time, and the assessment of the influence of temperature on the rate of reaction.
The rate of conversion, d
τ, is usually assumed to be a linear function of a single temperature-dependent rate constant, k, and a temperature-independent function of the conversion,
α, i.e., d
The quantitative representation of the rate-temperature dependence of k has been almost universally expressed by the Arrhenius equation, k = A.exp(-Ea/RT), where A is the “frequency factor” (usually assumed to be independent of temperature), Ea is the activation energy, and R is the ideal gas constant.
Values of the Arrhenius equation, or else the Arrhenius parameters Ea, the activation energy, and A (called also the “pre-exponential factor”) describe quantitatively the energy barrier to reaction and the frequency of occurrence of the situation that may lead to product formation, respectively. As such, these parameters facilitate the concise reporting of kinetic data, and the comparison of different systems from the point of view of their chemical reactivities. Moreover, they can be used to forecast behaviour at temperatures outside the intervals of different conditions of the experimental measurements.
The use of Arrhenius equation which has been applied to the study of the kinetics of homogenous reactions for some hundred years, was also extended to the thermal analysis of polymers.
The reactions that take place during the thermal decomposition of polymers are classified as heterogeneous. The question arises whether or not the validity of the Arrhenius equation may cope with such an extension, as the kinetics of homogenous and heterogeneous reactions are fundamentally different. In homogenous reactions, the reaction takes place at a uniform rate in every space unit of the single phase, while in heterogeneous reactions, the reactions takes place only on the phase boundaries of the contacting phases and at a rate permitted by the predominant mass and heat transport processes. The elementary chemical reaction taking place on the surface of the phase boundary is generally faster than the other elementary processes, and the course of transformations is usually defined by slow heat- and gas-transport processes, which are greatly influenced by experimental conditions.
Arnold et al.  noticed that the course of conventional thermoanalytical curves is more characteristic of the experimental conditions (the above-mentioned transport processes) than of the reaction itself. They conclude that the correctness of reaction kinetic calculations on the basis of curves obtained by dynamic thermoanalytical methods is rather questionable. However, if the experimental conditions are taken into account in appropriate way as to their further exploitation in kinetic analysis, this limitation can be overcome.
As Arnold et al.  noticed, the estimated parameter values are dependent on the mathematical methods used rather than on the thermoanalytical curve itself. But their affirmation that “It is shown experimentally that dynamic thermoanalytical curves provide insufficient information for the purpose of reaction kinetic calculations” seems to be rather exaggerative, as they estimate parameter triplets (A, E, n) from a single measured curve. No doubt that such calculations can lead to many deviating results while using different kinetic calculation methods. The standard practice that will be applied in this thesis is that the kinetic parameters estimation must be backed up not only by different kinetic calculation methods that complement themselves, but also by a set of curves measured in different experimental conditions, i.e. in the case of non-isothermal techniques, at various heating rates.
The methods of kinetic analysis of thermogravimetric data are divided into five categories (Flynn and Wall ): 1) “Integral” methods utilizing weight loss versus temperature data directly, 2) “Differential” methods utilizing the rate of weight loss, 3) “Difference-differential” methods involving differences in rate, 4) methods specially applicable to initial rates, and 5) nonlinear or cyclic heating rate methods.
In the next few paragraphs, the advantages and disadvantages of the first three methods will be briefly mentioned, as these groups are used most. A detailed description of the integral method applied in the thesis will be presented in the experimental protocol section dealing with the TGA data treatment methods.
In integral methods, results are less affected by experimental errors, as these methods evaluate the whole experimental data set and are based on the primary experimentally acquired data,
Differential methods based on rate of mass loss versus temperature data are much simpler in application and some of them are able to circumvent difficulties of many integral methods. However, they have a strong weakness: experimental noise is magnified, which renders the whole task of evaluating kinetic parameters very difficult, sometimes even impossible.
The difference-differential method of Freeman and Carrol and its modifications are the most widely used methods for the kinetic analysis of thermogravimetric data. It was used for the investigation of both inorganic materials and polymers. In general, one may obtain the initial parameters only if high accuracy data can be obtained at low conversions. The experimental noise, being magnified by interpreting the difference of a derivative, will not – in many cases – allow the determination of order at low conversion. As Flynn and Wall  have noted, these methods seem to be of limited applicability to polymeric systems with complex kinetics.
On the top of that, Ozawa  have found that the Freemann and Carroll, Coats and Redfern, and Sharp and Wentworth methods cannot be applied to a second-order reaction, random scission in main chains of polymers, and a system of two parallel competitive first-order reactions. As he pointed out: “… when one does apply them [i.e. the methods mentioned above] to these cases [the above-mentioned reactions], nearly straight relations are observed and false unreal kinetic parameters are obtained”. In
their kinetic parameters are false. Ozawa’s method, however, gives correct kinetic parameters. As Wendlandt  notes, one of the methods of avoiding false parameters is to observe a process at different heating rates. If the kinetic parameters estimated by analyzing the curves at different heating rates coincide with each other, the kinetic parameters are not false. He recommends also application of two or more methods to corroborate the resulting kinetic parameters. And as a most desirable way, he considers the use of a method based on a more fundamental kinetic equation, such as that of Ozawa .
Before entering the chapter on the subject matter of the theoretical study of individual polymers, the procedure employed in the experimental study will be presented. It consisted of:
1) choosing the conditions of pyrolysis convenient to a particular polymer,
2) conducting a set of experiments at chosen heating rates, usually repeating the same experiment three times,
3) simultaneously registering FTIR data during the whole experiment, with one scan about each 30 seconds,
4) evaluating infra-red spectra, correlating them with the assumed reaction history, 5) eventually carrying out the FTIR analysis of residues (systematically done only in the case of lignin, as there were no reference data found on other polymers or the specific study was not considered as a contribution from the point of view of theoretical and/or practical meaning),
6) calculating of kinetic parameters, according to the integral method presented in the sub-chapter entitled TGA data treatment (p. 62),
7) eventually evaluating of kinetic parameters by means of a MatLab program, making use of the differential method presented in the chapter mentioned above (point 6).
Below see a special chapter giving more details on issues concerning especially the so-called isothermal and non-isothermal kinetics. For a more exhaustive review of the problem, we invite the reader to kindly refer to the special section with selected references dealing with kinetics (section 6).
2.3.1 Isothermal vs. non-isothermal kinetics and other issues
As Vyazovkin  explains, for both isothermal and nonisothermal kinetics, the currently dominating approach appears to be force-fitting of experimental data to different reaction models. Following these indiscriminate model fitting methods, Arrhenius parameters are determined by the form of f(
α) chosen. Such methods tend to fail to meet even the justifiable expectations. The application of these methods to isothermal data gives rise to believable values of Arrhenius parameters that, however, are likely to conceal the kinetic complexity. In a nonisothermal experiment both T and
αvary simultaneously. The application of the model-fitting approach to single heating-rate data generally fails to achieve a clean separation between the temperature dependence, k(T), and the reaction model, f(
α). As a result, almost any f(
α) can satisfactorily fit the data at the cost of drastic variations in the Arrhenius parameters, which compensate for the difference between the assumed form of f(
α) and the true but unknown reaction model. For this reason, the application of the model-fitting methods to single heating-rate data produces Arrhenius parameters that are highly uncertain and, therefore, cannot be meaningfully compared with the isothermal values. Unfortunately, for years, the model-fitting analysis of single heating rate data has been the most prevalent computational technique in nonisothermal kinetics. That is why the failures of this technique have been mistaken for the failures of nonisothermal kinetics as a whole. Vyazovkin  points out that an alternative approach to kinetic analysis is to use model-free methods that allow for evaluating Arrhenius parameters without choosing the reaction model. The best known representatives of the model-free approach are the isoconversional methods. These methods yield the effective activation energy as a function of the extent of conversion. Knowledge of the dependence Ea on
αassists in both detecting multi-step processes and drawing certain mechanistic conclusions. Secondly, it is sufficient to predict the reaction kinetics over a wide temperature region. Thirdly, the isoconversional methods yield similar (but not identical!) dependences of the activation energy on the extent of conversion for isothermal and nonisothermal experiments.
He stipulates that fitting data to reaction models cannot be used as the sole means of identifying the reaction mechanisms. Note that this is equally true in the case when
statistical analysis allows one to unequivocally choose a single reaction model – statistical analysis evaluates the reaction models by the goodness of fit of the data, but not by the physical sense of applying these models to the experimental data. Even if a reaction model does not have any physical meaning at all, it may well be the best fit to the experimental data.
According to Vyazovkin, the most important feature of a reliable method of kinetic analysis is its ability to handle multi-step processes that are rather typical for reactions of solids. He founds the model-free and model-fitting methods that use sets of isothermal or/and nonisothermal data obtained at different temperatures or/and at different heating rates to be very effective in detecting this feature in the data provided. The model-free methods reveal the kinetic complexity in the form of a dependence of the activation energy on the extent of conversion (isoconversional methods) or in the form of a temperature dependence (the NPK method) – the ‘non-parametric kinetics’ method of Nomen and Sempere [Serra, 1998]. While too young to reveal all the ups and downs, the NPK method makes a promising debut. It is easy to appreciate the value of the isoconversional method, which is a seasoned veteran of kinetic battles. As seen from the results of the project, various isoconversional methods applied by different workers to the same set of nonisothermal data have produced consistent dependences of the activation energy on the extent of conversion. This fact bears a great meaning for nonisothermal kinetics that for years has been a subject of acidulous criticisms and humiliating mockery for its alleged inability to produce sensible kinetic data. The isoconversional methods may also be helpful in providing some mechanistic clues. … the mechanistic clues are not yet the reaction mechanism, but rather a path to it that can further be followed only by using species-specific experimental techniques.
According to Vyazovkin , the isoconversional method of Friedman presents the most straightforward way to evaluate the effective activation energy, Ea, as a function of the extent of reaction. This is a differential method, which can be applied to integral data (e.g. TG data) only after their numerical differentiation. As we have indicated before (in the paragraph about differential methods), because this procedure may lead to erroneous estimates of the activation energy, the use of the integral isoconversional methods appears to be a safer alternative.
The consistency of the kinetic parameters derived from isothermal and nonisothermal data should not be used, as it follows from Vyazovkin’s analysis, as a decisive criterion to determine if the values are trustworthy. It is not a sufficient condition. He exemplifies this on the fact that although fitting isothermal and nonisothermal data to single-step models resulted in incorrect values of the kinetic triplets, the latter are also in perfect agreement.
Vyazovkin  further shows that there are some rather insignificant differences between the Ea-dependences obtained by using integral and differential methods. These differences arise partially from the fact that the equations of the integral methods are usually derived under the assumption of the constancy of the activation energy. On the other hand, the differential methods may suffer from imprecise numerical differentiation, even in the case of artificial data that are free of ‘experimental noise’.
In conclusion, he declares that model-free techniques have been very successful in detecting multi-step kinetics in the data provided. Fitting data to multi-step kinetic models has allowed the ‘true mechanism’ to be guessed for the simulated data. For the real data, the mechanistic guesses happened to be uncertain. The fact that the obtained Ea-dependences allow one to unmistakably recognize a multi-step process taken alone is, according to him, already a very important piece of mechanistic information.
Brown et al.  say that use of small samples has decreased the problems of heat transfer at the expense of a possible decrease in the homogeneity of the sample.
On the assumption that the data obtained are reliable and that random noise in the data is negligible, one can proceed in the search for a mathematical description of the data.
A mathematical description of the data is usually sought in terms of a ‘kinetic triplet’ (i.e. Arrhenius parameters A and Ea, and the reaction model, f(
α), also called the conversion function).
Attempts have to be made to relate the computational results to the actual sequence of physico-chemical processes occurring, i.e. the reaction mechanism. Formulation of such a relationship is generally only possible with the aid of complementary information from microscopic, spectroscopic and structural studies.
The ability to handle multi-step reaction mechanisms is a desirable feature of a computational method. Multi-heating rate and isoconversional methods have proven to be particularly effective and most of the recent interest in the field of kinetic computations has been concerned with these methods.
The goodness of fit is only the necessary, but not the sufficient condition for the identified reaction model to be physically sound.
Maciejewski  demonstrates by experimental data that the kinetic description of the process depends strongly on the experimental conditions. The very limited applicability of the kinetic methods that use single-heating rate data is emphasized.
Direct comparison of the kinetic parameters obtained by different computational methods is very problematic because it is unclear whether the observed differences in the values originate from differences in the experimental conditions of from the differences in the computational methods.
(Project provides a unique opportunity to compare computational methods, because different methods are applied to the same sets of experimental and simulated data.)
The kinetic description of the solid state reactions is influenced not only by the complicated nature of the process but also by the method of calculation.
Besides, we cannot choose ‘the best’ method, because we do not know the correct mechanism and kinetic parameters. This is possible only for simulated data for which the kinetics triplets are known exactly.
Only computational methods, which use multi-heating rate data, can produce a reliable mathematical description of the reaction kinetics. The methods that use single heating rate data should simply be avoided in serious kinetic analyses.
He further notes that the dependence of Ea on
αis observed when a process involves several steps that have different activation energies. There is, however, a danger of missing the multi-step character of a process in the case when different steps have practically equal activation energies, but have different pre-exponential factors and/or obey different kinetic models.
In real experiments, there are two reasons that can prevent consistent kinetic triplets from isothermal and non-isothermal data being obtained: (i) the temperature ranges of isothermal and non-isothermal experiments are not the same; (ii) truly isothermal
conditions cannot be accomplished for the very low and very high ranges of the reaction extent
Isothermal experiments cannot be carried out at temperatures when the reaction rate is too fast and significant decomposition may occur during settling of the experimental temperature at the beginning of the experiment. This undefined period depends upon the experimental conditions (applied temperature ramp, sample mass, the kind of carrier gas) and reactant properties (cp, thermal conductivity, the mechanism of the decomposition) and makes it experimentally impossible to achieve strictly isothermal conditions over the full range of conversion. For many kinetic models the maximum rate of decomposition, under isothermal conditions occurs at the beginning of the reaction.
As far as non-isothermal experiments, he noticed difficulties of the determination of the
α-T dependence at the beginning of the decomposition. Due to the specific shape of this dependence for some functions, especially for the contracting geometry and diffusion models, the change of the reaction progress from 0.001 to 0.02 required, at a heating rate of 5 K.min-1, the temperature change of 63 K (R2) or 109 K (D3), respectively. Due to buoyancy effects, the determination of such small mass changes over a relatively long period of time is uncertain.
Another important factor that affects the reliability of kinetic data obtained for very low and very high a values is self-heating/cooling. The distortion of the preset temperature program is especially high at the beginning of isothermal and at the end of non-isothermal experiments due to the occurrence of the greatest thermal effects at these stages of the process. The effect of self-heating/cooling increases with increasing sample mass. The deviation of the actual T from the preset temperature may invalidate any evaluation of the kinetics triplets.
Comparison of the kinetic parameters obtained under isothermal and non-isothermal conditions is aggravated by unavoidable experimental phenomena that affect the kinetic data. In the case of a relatively simple process, whose kinetics can be described by a single kinetic triplet, the difference is primarily determined by these experimental phenomena, but not by computational methods (provided they are valid).
In the narrower ranges used under iso-thermal conditions, the difference between different models are much less visible.
The solution for avoiding these problems would seem to be the opposite procedure: determination of kinetic parameters should be done from non-isothermal experiments carried out over a wide temperature range.
The results of experiments carried out indicate that the same process cannot be characterized by the same kinetic triplet under different experimental conditions.
As a first test for reaction complexity, one should use isoconversional methods. The complexity is easily detectable as a variation of the activation energy with
In a real system, the influence of the experimental conditions disturbs, in a different way, the course of the isothermal and non-isothermal dependencies, …, making the comparison of isothermal and non-isothermal kinetic parameters more difficult. Due to the fact that non-isothermal parameters are calculated from the data obtained in a much wider temperature range, it is logical to use them for the prediction of isothermal runs. The opposite procedure, i.e. the prediction of non-isothermal relationships based on the isothermal parameters may be erroneous.
He thinks it proven that the original isoconversional methods (Ozawa, Friedmann) are very sensitive to experimental noise which leads, despite their mathematical simplicity, to a great scatter of the results, etc.
In Burnham’s  opinion, isoconversional methods give kinetic parameters that agree qualitatively with those from subsequent nonlinear regression to appropriate models. Single-heating-rate methods work poorly and should not be used or published. He summarizes his contribution to the ICTAC kinetics projects in these words: the isoconversional analyses of various workers tend to agree fairly well and give qualitatively good predictions of the activation energies ultimately obtained from non-linear regression to appropriate models.
He found that the isoconversional methods give a narrower set of results and uniformly agree that the activation energy decreases during conversion.
According to him, the isoconversional analyses of various workers tend to agree fairly well and give qualitatively good predictions of the activation energies ultimately obtained from non-linear regression to appropriate models.
As is also recommended in a recent material by the ICTAC [Roduit 2000], the computations should be carried out with experimental data obtained from at least two or three different heating rates (non-isothermal) or temperatures (isothermal). Moreover, the data should be collected under similar experimental conditions because the kinetic parameters of solid-state reactions are not intrinsic properties of an investigated compound, but can change depending on the experimental conditions applied. This is known as PSTA-principle or parametric sensitivity of thermal analysis [Roduit et al. 1996].
Isoconversional methods are known to allow the calculation of model-independent estimates of the activation energy, E(
α), related to different extents of conversion,
In 2000, a series of 5 papers was published containing the results of an ICTAC kinetics project. Besides the model-fitting analysis, most of the participants have tried to recover the hidden activation energies by applying isoconversional methods (Friedman, Ozawa-Flynn-Wall). The kinetics results computed for a hypothetical simulated process and experimental data for the thermal decompositions of calcium carbonate and ammonium perchlorate were presented. The comparison of the kinetic parameters obtained from isothermal and non-isothermal (a.k.a. „dynamic“) experiments was presented and discussed. Experiments were carried under vacuum and nitrogen. In Part E, dealing with numerical techniques and kinetics of solid state processes, Roduit  commented that measurements of experimental data carried out under isothermal conditions are usually investigated in a narrow temperature range due to technical problems. Therefore, they may not contain the information necessary for determining the complexity of a process. He stated also that the use of heating rates which are higher than 2-3 K.min-1 helps to discern between the different reactions involved in the kinetic scheme. In his experiments, he found that if heating rates are too similar, they narrow the temperature region of non-isothermal experiments, and model-fitting analysis becomes comparable to that using single heating-rate methods and may fail to determine the best kinetic models, just as for isothermal experiments carried over a narrow range of temperatures. He argued that consideration of the wide range of temperatures achieved with non-isothermal experiments provides very important insights in interpreting and